Section 22.214.171.124 states: “The HRC method may be used for welding procedure qualification. . . And the welding procedure specification includes post-weld heat treatment” and Clause A.2.1.4 states: “As-welded carbon steels, carbon manganese steels and low alloy steels that comply with the hardness requirements of Table A.1 do not require postweld heat treatment.” It is confusing whether the latter statement implies that an as-welded carbon steel, carbon manganese steel, or low alloy steel would require a PWHT if only HRC hardness testing is performed. Per Section 126.96.36.199, I would say yes it does require PWHT. But if the as-welded hardness survey meets the 22 HRC limit then doesn’t the as-welded material “comply with the hardness requirements of Table A.1 as stated in clause A.2.1.4?
For carbon, carbon manganese, and low alloy steels hardness testing for welding procedure qualification (PQR) may be performed by the HRC method only if the design stress does not exceed 2/3 SMYS and PWHT is perform. If PQR hardness testing is performed by the 188.8.131.52 specified HV or HR15N methods, the restrictions for design stress and PWHT are not required.
This question is in relation to NACE MR0175/ISO 15156-2 Clause 184.108.40.206
Reference: ISO 15156 Maintenance Panel Inquiry #2011-14
Contact us to discuss the NACE MR0175 requirements and your welding procedure qualification, we are here to help.
With a wealth of experience in the oil and gas industry, we provide independent materials and corrosion consultancy to help companies reduce risk, save money and apply best practice in their oil and gas businesses.
Find out more by getting in touch – you’ll get an answer from a qualified, experienced materials engineer every time.
How to get in touch
US: 877-399-1010 (toll free)